doi:10.4236/msa.2011.27114 Published Online July 2011 (http://www.SciRP.org/journal/msa)
Dielectric Behaviour of Pure and Dye Doped
Nematic Liquid Crystal BKS/B07
Rajiv Manohar2, Shashwati Manohar3, V. S. Chandel1
1Department of Physics, Integral University, Lucknow, India; 2Department of Physics, Lucknow University, Lucknow, India; 3Department of Physics, RML Awadh University, Faizabad, India.
Received July 26th, 2010; revised September 4th, 2010; accepted May 30th, 2011.
The dielectric properties of pure nematic liquid crystal (BKS/B07) and dye doped (Rhodamine B and Anthraquinone) nematic liquid crystal have been investigated in a wide frequency range of 1 kHz to 10 MHz through the dielectric spectroscopic method at varying temperature. In addition to this optical transmittance and textures of the samples have also been observed with a polarizing microscope.
Keywords: Liquid Crystals, Dielectric Properties
Organic molecules and liquid crystals (LC) are well es-tablished materials for photonic and non-linear optical device applications because of their optical non linearity and very rapid optical response . In a mixture of LC and dichroic dye the action of an electric field influences the collective orientation of the LC molecules and that of the dye molecules. This phenomenon is called Guest-host interaction. Dyes have been widely used as guest addi-tives in optical materials to develop novel optoelectronic devices. Again it is well established that the presence of dye molecules in the liquid crystal host influences many properties of the pure liquid crystals. The Effect of dye on dielectric properties of liquid crystals has been inves-tigated earlier by some groups [2,3]. The change in nonlinear refractive index and birefringence of dye doped nematic mixture has been investigated by A. Jafari et al.. It has also experimentally proved that doping a small amount of dye decreases the required threshold of molecular reorientation further in LC materials . Temperature dependence of direction reorientation of dye doped nematic liquid crystal has been studied by Esteves et al. . Voigot et al. have studied emission of circularly polarized light in dye based chiral nematic liquid crystals . Thermal non-linearity of dye doped nematic liquid crystals have been reported by Henninot et al. , while photovoltaic effect in liquid crystal cells containing dyes have been studied by Sato et al. . Mustafa Okutan et al. have studies refractive index
dis-persion and electrical properties of carbon nono –balls’ doped nematic liquid crystal .
Most of the efforts are aimed on the electro-optical characterization of LC [11,12], but no serious work have been done in understanding the dielectric properties of dye doped liquid crystals. In the recent years few articles have been published by Mustafa Okutan et. al., S. Ozder et al. [13-15].The dielectric spectroscopy technique has also been used by many workers for the study of LCs in different phases, as the technique provides very accurate data about the material under investigation. Therefore, the present paper is an effort to investigate the effect of dye on dielectric property of liquid crystal host mole-cules. In order to confirm the changes occurred in phase transition temperature as a result of dye mixing optical transmittance measurement of the sample have also been done.
The liquid crystal sample used for the present investiga-tion was used without further purificainvestiga-tion. The transiinvestiga-tion schemes of the pure sample as well as dye doped samples are as follows: (Figure 1)
All dyes used in the experiment were obtained from Thomas Beker. Their chemical names and compositions are given below. (Figure 2)
Crystalline 126 C Nematic 130 C Isotropic
Nematic sample doped with anthraquinone dye
Crystalline 121 C Nematic 125 C Isotropic
Nematic sample doped with rhodamine B dye
Crystalline 122 C Nematic 126 C Isotropic
Figure 1. Structure of Nematic sample BKS/B07.
1,5- Diamino-2(4-heptyloxy-phenyl)-4,8-dihydroxy-anthraquinone CHEMICAL COMPOSITION: C27 H23 N2 O5
Rhodamine B Dye
N-[9-(2-Carboxyphenyl)-6-(diethylamino)-3H-xanthen-3-ylidene]- N-ethylethanaminium chloride
CHEMICAL COMPOSITION: C28 H31 ClN2 O3
N+ O N
6 8 10 12 14 16 18
3 4 5
6 8 10 12 14 16 18
2 3 4 5 6 7 8
6 8 10 12 14 16 18
4 5 6 7 8
Pure BKS/B07 12 C60
log10 of Frequency
'BKS/B07 doped with anthraquinone dye
BKS/B07 doped with rhodamine B dye 1240
Figure 3. Variation of dielectric constant with log10 of frequency for pure nematic sample with two dyes (anthraquinone,
6 8 10 12 14 16 18
2 6 8 10 12 14 16 18
0 1 2
3 6 8 10 12 14 16 18
0 1 2 3
Pure BKS/B07 128
log10 of Frequency
BKS/B07 doped with anthraquinone dye 1240C
BKS/B07 doped with rhodamine B dye 1240C 1250C
Figure 4. Variation of dielectric loss with log10 of frequency for pure nematic sample with two dyes (anthraquinone,
sample of BKS/B07 was prepared in the lab by disper-sion of two dyes under investigation at a concentration of about 2% wt/wt in the liquid crystal host material. The strong interaction between two different types of mole-cules allow the samples to maintain a good alignment , which has been confirmed by observing at the sam-ple holder under polarizing microscope. This guest-host mixture and pure sample were filled in a sandwich type sample holder having coating of Indium Tin Oxide (ITO) on the glass substrate and pre-treated with polyamide for planner type alignment. The temperature of the sample was controlled and maintained by a microprocessor based temperature controller Julabo (model no. F-25 HD) to an accuracy of 0.01˚C. The temperature of the sam-ple holder on the double walled jacket was measured using an external Pt-100 type sensor. The sample cell was connected to Hewlett-Packard Impedance/Gain Phase Analyser (model HP 4194 A) working in the fre-quency range of 1 kHz to 40MHz. For obtaining the val-ues of capacitance and dissipation factor, the sample holder was calibrated using AR grade benzene. The val-ues of capacitance in the cell with sample and without sample were measured. The dielectric constant was ob-tained using the relation
where ∆C is change in capacitance of the sample holder with and without sample, which is
C C C
(2) where CP is the capacitance of sample holder with sample and C0 is the capacitance of sample holder without sample. is the geometrical capacitance of the sample holder. G
For the measurement of dielectric loss, dissipation factor D was measured for the sample holder with and without sample. Thus, the loss tangent was obtained us-ing the relation
tan P P O O
C D C D
where DP and O are the dissipation with and
with-out sample respectively. D
Dielectric loss was determined using relation
ε= εtanδ (4) For the measurement of optical transmittance, a preci-sion research polarising microscope was used (model no. CENSICO 7626). The homogeneously aligned sample holder was placed on a hot stage which is a double walled chamber in which oil of required temperature was circulated. For variation of temperature, the same tem-perature controller Julabo (model no. F-25 HD) as used
during dielectric measurements was again used. The hot stage was placed between cross polarisers in the polaris-ing microscope. The aligned sample was placed between crossed polarisers and was heated and the emergent light at different temperature was made to incident on one of the eyepieces which is fitted with a light dependent re-sistance (LDR). Thus, the variation of emergent light varies the resistance of LDR, which directly provides us the optical transmittance in arbitrary units.
Textures (microphotographs) of the samples have also been taken using a polarising microscope which is fitted with a camera in one of its eye pieces.
4. Results and Discussion
The variation of real and imaginary parts of relative per-mittivity, that is dielectric constant () and dielectric loss () for pure nematic sample BKS/B07 and two dye mixed samples with log of frequency are shown in Fig-ures 3 and 4 respectively. The variation of real and imaginary parts of relative permittivity that is dielectric constant () and dielectric loss () for pure nematic sample BKS/B07 and with two dyes anthraquinone (mixture 1) and rhodamine B (mixture 2) with tempera-ture are shown in figures 5 and 6 respectively. Figure 7 shows the variation of percentage optical transmittance with temperature for pure nematic sample BKS/B07 and two dye mixed samples (mixture 1 and 2). Textures of the nematic sample BKS/B07 along with its two guest-host mixtures in crystalline and nematic phases have been presented in Figures 8 to 9.
The dielectric parameters and have been meas-ured for a nematic liquid crystal BKS/B07 in the fre-quency range of 1 kHz to 10MHz for the temperature range of 70˚C to 135˚C. Figure 3 and Figure 4 represent typical frequency dependence spectra of the real and imaginary part of the dielectric permittivity measured for nematic sample BKS/B07 and dye doped mixtures 1 and 2. The dielectric permittivity is found to be either con-stant or to decrease as the frequency increases [17-22] for pure sample. Lower values of at higher frequency suggest that the molecules rotate about their long mo-lecular axis . The behaviour of for the dye based mixtures 1 and 2 is similar to that of pure sample but the values of dielectric constants are higher in comparison to the corresponding values of pure sample.
One can see from the figure 4 that a maximum in the loss curve is observed at frequency 382 kHz for the tem-perature 128˚C for pure sample. The peak in the curve indicates dielectric relaxation and it shifts towards lower side of frequency as the temperature increases as ex-pected and also reported by other workers [24,25].
100 110 120 130 3.2
100 110 120 130 140
4.0 4.4 4.8 5.2
100 110 120 130 140
4.0 4.4 4.8 5.2 5.6 6.0
100 KHz 200 KHz
100 KHz 200 KHz BKS/B07 doped with rhodamine B dye
BKS/B07 doped with anthraquinone dye 100 KHz 200 KHz
Figure 5. Variation of dielectric constant with temperature for pure nematic samplewith two dyes ( anthraquinone, rhoda-mine B).
100 110 120 130 140
100 110 120 130 140
100 110 120 130 140
100 KHz 200 KHz
BKS/B07 doped with rhodamine B dye
100 KHz 200 KHz BKS/B07 doped with anthraquinone dye
100 KHz 200 KHz
100 105 110 115 120 125 130 135 140 0
10 20 30 40 50
60100 105 110 115 120 125 130 135 140
0 10 20 30 40 50 60 70
80100 105 110 115 120 125 130 135 140
0 10 20 30 40 50 60 70 80
BKS/B07 doped with anthraquinone dye BKS/B07 doped with rhodamine B dye
Figure 7. % Inverse Optical transmittance Vs temperature for pure nematic samplealong with two dyes ( anthraquinone, rhodamine B).
Figure 8. Texture of pure nematic sample BKS/B07 in (a) crystalline phase at 80˚C; (b) nematic phase at 127˚C.
Figure 10. Texture of Pure nematic Sample BKS/B07 doped with rhodamine B dye in (a) crystalline phase at 80˚C;(b) nematic phase at 123˚C.
from the Figure 4 that the peak of the curve has been significantly shifted from the frequency of the peak ob-tained for pure sample. It suggests that the relaxation frequency of the dye doped mixture is different from that of pure sample and variation also depends upon the type of dye used and its compatibility with the liquid crystal host.
The variation in the value of and due to addition of dye can be explained by considering the contribution of dipole moment of dye molecule in the host liquid crystal molecule. Each dye molecule has a preferential axis of orientation and it will get aligned along the host liquid crystal molecule thereby resulting in the restriction on the freedom of its movement. Thus, the dipole mo-ment of dye molecule contributes significantly to the actual value of and and also relaxation frequency value .
The Figures 5 and 6 show the variation of and as a function of temperature for nematic sample BKS/B07 and for mixtures 1 and 2. For the frequency range 1 kHz –10 MHz, the dielectric constant remains almost constant for the crystalline region and crystalline to nematic tran-sition is detected by slight variation of dielectric constant at 126˚C for nematic sample BKS/B07. It is interesting to note that a sharp peak appears near nematic to isotropic transition temperature at 130˚C whose magnitude in-creases with dein-creases in the frequency. This type of variation has also been reported by other workers for other type of samples . Similar types of variations have been noticed for the curves of versus temperature at varying frequencies shown in figure 6. The hump at the nematic to isotropic phase transition temperature is more clear for lower frequencies.
The variation of and with temperature for guest-host mixtures also have similar nature with a change that the transition temperature have shifted to-wards lower side by about 4˚C to 5˚C in comparison to the transition temperature for pure samples . The transition temperature for mixture 1 are 121˚C and 125˚C
for crystalline to nematic and nematic to isotropic transi-tion. While for the mixture 2 the values of transition temperatures are 122˚C and 126˚C for the two transitions respectively. This decrease in the transition temperature is due to the fact that dye molecules behave as an impu-rity molecule in the liquid crystal host. The presence of impurity definitely decreases the transition temperature of the sample. It has been reported by our group  and various other researchers. Also the increased breadth of transition suggests that dye molecules behave as im-purity in the liquid crystal matrix .
pos-sible that the dye molecules are behaving like impurity molecules for liquid crystal host. The breadth of the nematic-isotropic phase has also been observed by De-mus et al.  and Singh et al.  for mixtures. It may be concluded that sharpness of the transition depends upon purity of the sample and it increases with the addi-tion of different components because they behave like impurity with respect to each and that might be the rea-son for existence of bi-phase region. The phase transition temperatures as obtained by dielectric measurement technique and optical transition measurement technique are found to be very close to each other.
Textures (microphotographs) of pure sample and their guest host mixtures are shown in Figures 8(a, b), 9(a, b) and 10 (a, b) in crystalline and nematic phases. It may be seen that these textures also support our observations of the existence of different phases and identification of phase transitions [33-37].
It may be concluded that dielectric constant and dielec-tric loss values increase with the addition of dye and the relaxation frequency shift towards the lower or higher side depending upon nature, structure of dye and com-patibility with the liquid crystal host. The transition tem-perature shifts towards lower side with the addition of dye because the guest molecule behaves like impurity for the pure sample. The absorption of light increases sig-nificantly due to presence of guest dye molecule in host liquid crystal molecule.
Authors are thankful to Prof. B. K. Sadashiva of Ra-man Research Institute, Bangalore, India for providing the nematic sample. Authors are also thankful to ISRO for grant funds in the form of project.
 K. Y. Wong, A. K.-Y. Jen, V. P. Rao and K. J. Drost, “Theoretical and Experimental Studies of the Molecular Second Order Nonlinear Optical Responses of Het-eroaromatic Compounds,” Journal Chemical Physical, Vol. 100, January 1994, pp. 6818-6825.
 D. Bauman and W. Haase, “Dielectric Measurements of Guest-Host Systems,” Molecular Crystals Liquid Crystals, Vol. 168, August 1989, pp. 155-168.
 D. Bauman, “Comparative Studies of the Degree of Order of the Guest and Host Molecules in 4-Cyano-4'-n- Hep-tylp-Phenylcyclohexane (PCH7) Mixtures,” Molecular Crystals Liquid Crystals, Vol. 174, March 1989, pp. 1-10.
 A. Jafari, H. Tajalli and A. Ghanadzadeh, “The Effects of External Applied Voltage on the Nonlinear Refractive Index and the Birefringence of a Dye-Doped Nematic
Mixture,” Optics Communication, Vol. 266, No. 1, April 2006, pp. 207-213. doi:10.1016/j.optcom.2006.04.050
 F. Simoni and O. Francescangeli, “Effects of Light on Molecular Orientation of Liquid Crystals,” Journal Physical Condensed Matter, Vol. 11, No. 41, October 1999, pp. 439-487. doi:10.1088/0953-8984/11/41/201
 J. Esteves and A. M. Figueiredo Neto, “Temperature De-pendence of the Director Reorientation of Dye-Doped Nematic Liquid Crystals Subjected to an Optical Field And its Relation with the Non-Linear Absorption Coeffi-cient,” Liquid Crystals, Vol. 29, No. 5, May 2002, pp. 733-742. doi:10.1080/02678290210127760
 M. Voigt, M. Chambers and M. Grell, “Circularly Po-larized Emission from a Narrow Bandwidth Dye Doped into a Chiral Nematic Liquid Crystal,” Liquid Crystals, Vol. 29, No. 5, May 2002, pp. 653-656.
 J. F. Henniot, M. Dehailleul and M. Warenghem, “Tun-able Non-locality of Thermal Non-linearity in Dye Doped Nematic Liquid Crystal,” Molecular Crystals Liquid Crystals, Vol. 375, May2002, pp. 631-640.
 S. Sato and S. Fukudo, “Photovoltaic Effects in Liquid Crystal Cells Containing Organic Dyes,” Molecular Crystals Liquid Crystals, Vol. 98, February 1983, pp. 99-108. doi:10.1080/00268948308073465
 M. Okutan, S. E. San, O. Koysal and F. Yakuphanoglu, “Investigation of Refractive Index Dispersion and Elec-trical Properties in Carbon Nano-Balls’ Doped Nematic Liquid Crystals,” Physica B, Vol. 362, No. 1-4, February 2005, pp. 180-186.
 H. Allinson and H. F. Gleesson, “Dielectric Permittivity Properties of a Fulgide Dye Guest-Host Liquid Crystal,”
Liquid Crystals, Vol. 19, No. 4, October 1995, pp. 421- 425. doi:10.1080/02678299508032002
 T. Grudniewski, J. Parka, R. Dabrowski, A. Januszko and A. Miniewicz, “Investigations of the Diffraction Effi-ciency in Dye Doped LC Cells under Low Frequency AC Voltage,” Opto-Electron Reviews, Vol. 10, No. 1, January 2002, pp. 11-15.
 M. Okutan, F. Yakuphanoglu, S. E. San and O. Koysal, “Impedance Spectroscopy and Dielectric Anisotropy-Ty- pe Analysis in Dye-Doped Nematic Liquid Crystals Hav-ing Different Preliminary Orientations,” Physica B, Vol. 368, No. 1-4, July 2005, pp. 308-317.
 M. Okutan, S. E. San and O. Koysal, “Dielectric Spec-troscopy Analysis of Molecular Reorientation in Dye Doped Nematic Liquid Crystals Having Different Pre-liminary Orientation,” Dyes and Pigments, Vol. 65, No. 2, September 2005, pp. 169-174.
 W. M. Gibbons, P. J. Shannon, S. T. Sun and B. J. Swet-lin, “Surface-Mediated Alignment of Nematic Liquid Crystals with Polarized Laser Light,” Nature, Vol. 351, May 1991, pp. 49-50.
 A. Agrawal, V. P. Arora, R. V. Kaushik, P. P. Anand, K. Agarwal and B. Bahadur, “Dielectric Relaxation Mecha-nism in Liquid Crystalline Mixture ZLI 1840,” Journal of Pure and Applied Physical, Vol. 27, 1989, pp. 299-301.  A. M. Biradar, S. Hiller, S. A. Pikin and W. Haase,
“Sur-face Molecular Relaxation in Smectic C* Phase as Stud-ied by Dielectric Spectroscopy,” Liquid Crystals, Vol.20, No. 2, October 1996, pp. 247-251.
 S. K. Kundu, K. Suzuki and B. K. Chaudhri, “Effect of Biasing Field on the Soft Mode in the Vicinity of the Smc*-Sma Phase Transition of a Ferroelectric Liquid
Crystal ZLI 4851,” Journal Applied Physical, Vol. 94, No. 4, August 2003, pp. 2271-2276. doi:10.1063/1.1587871
 H. J. Müller and S. JayaRaman, “Dielectric Properties of Nematic and Ferroelectric Liquid Crystals,” Molecular Crystals Liquid Crystals, Vol. 309, January 1998, pp. 93-110.
 A. K. Thakur, D. K. Sharma, S. P. Singh, S. S. Bawa and A. M. Biradar, “Dielectric Relaxation near the Transition Temperature of Sm C*-Sm A Phase in Electroclinic Liq-uid Crystal,” Ferroelectrics, Vol. 289, No. 1, January 2003, pp. 63-75.doi:10.1080/00150190390221160
 P. G. Cummins, D. A. Dunmur and D. A. Laidler, “The Dielectric Properties of Nematic 44’n-pentylcyanobipheny- l,” Molecular Crystals Liquid Crystals, Vol. 30, January 1975, pp. 109-123. doi:10.1080/15421407508082846
 A. M. Biradar, D. Kilian, S. Wrobel and W. Haase, “A Sub-Hertz Frequency Dielectric Relaxation Process in a Ferroelectric Liquid Crystal Material,” Liquid Crystals, Vol. 27, No. 2, September 2000, pp. 225-231.
 D. Bauman, J. Solczynski and E. Chrzumnicka, “Guest Effect on Nematic-Isotropic Phase Transition Temperatu- re of Liquid Crystal 6CHBT,” Liquid Crystals, Vol. 92, No. 6, August 1997, pp. 1155-1161.
 D. M. Potukuchi, A. George, C. Carboni, S. A. Harthi, J. Naciri, “Low Frequency Dielectric Relaxation, Spontane- ous Polarization, Optical Tilt Angle and Response Time Investigations in a Flourinated Ferroelectric Liquid Crys-tal, N125F2(R*),” Ferroelectrics, Vol. 300, No. 1, Janu-ary 2004, pp. 79-93. doi:10.1080/00150190490442245
 B. Bahadur, “Liquid Crystals-Application and Uses (vol-2),” World Scientific Publishing, NowYork, 1990.
 A. K. Srivastava, A. K. Mishra, P. B. Chand, R. Manohar and J. P. Shukla,” Shifting of Transition Temperature of Ferroelectric Liquid Crystals Due to Addition of Dye-An optical and Dielectric Study,” Journal of Physical Chemical Solid USA, Vol. 68, January 2007, pp. 523-529.
 A. K. Singh, R. Manohar; J. P. Shukla and A. M. Biradar, “Refractive Indicies, Order Parameter and Optical Transmittance Studies of a Nematic Liquid Crystal Mix-ture,” Acta Physica Polonica A, Vol. 110, No. 4, August 2006, pp. 485-496.
 R. Manohar, M. Gupta and J. P. Shukla, “ Phase Transi-tion Studies of Some Cholesteric Liquid Crystals and Their Mixtures Using Dielectric, Optical Transmittance and Density Measurement Studies” Journal of Pure and Applied Physical, Vol. 61, July 2000, pp. 1465-1473.
 F. M. Gouda, “Dielectric Relaxation Spectroscopy of Chiral Smectic Liquid Crystals” Ph.D. Dissertation, Dept. of Physics, Chalmers University of Technology, Gote-borg, Sweden, 1992.
 D. Demus, H. G. Hahn and F. Kuschel, “Density Meas-urements in Cholesteryl Myristate,” Molecular Crystals Liquid Crystals, Vol. 44, January 1978, pp. 61-70.  R. Singh, V. K. Agrawal, P. P. Anand and V. P. Arora,
“Optical Behaviour of Nematic Mixture: 1975/S,” Nature Academic Science Letters India, Vol. 13, No. 4, April 1990, pp. 129-131.
 M. B. Pandey, R. Dhar, V. K. Agarwal, R. Dabrowski and M. Tykarska, “Study of Different Modes of Dielectric Relaxation in a Newly Synthesized Material Exhibiting Ferro-, Ferri- and Antiferro-Electric Phases,” Liquid Crystals, Vol. 31, No. 7, July 2004, pp. 973-987.
 A. Sasaki, M. Inodo and T. Ishibashi, “Light Transmissi- on and Texture Changes of Mixed Liquid Crystals by Temperature Variations,” Molecular Crystals Liquid Crys-tals,Vol. 65, February 1981, pp. 39-49.
 E. G. Hanson and Y. R. Shen, “Refractive Indices and Optical Anisotropy of Homologous Liquid Crystals,”
Molecular Crystals Liquid Crystals, Vol. 36, March 1976, pp. 193-207. doi:10.1080/15421407608084323
 P. G. de Gennes, “The Physics of Liquid crystals,” 3rd Edition, Clarendon Press, Oxford, 1974.